#------------------------------------------------------------------------------
#$Date: 2016-03-26 16:01:19 +0100 (Sat 26 de Mar de 2016) $
#$Revision: 180368 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/37/7203770.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7203770
loop_
_publ_author_name
'León-Reina, Laura'
'Losilla, Enrique R.'
'Martínez-Lara, Maria'
'Bruque, Sebastián'
'Llobet, Anna'
'Sheptyakov, Denis V.'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Interstitial oxygen in oxygen-stoichiometric apatites
;
_journal_issue                   25
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2489
_journal_paper_doi               10.1039/b503374h
_journal_volume                  15
_journal_year                    2005
_chemical_formula_sum            'Ge La1.33 O4.33 Sr0.33'
_chemical_formula_weight         356.33
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_audit_creation_date             2004-06-11T10:29
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2004-06-11T10:29 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.9422(6)
_cell_length_b                   9.9422
_cell_length_c                   7.3358(4)
_cell_volume                     627.98(5)
_computing_structure_refinement  GSAS
_pd_block_id
2004-06-11T10:29|LA8SR2GE6_675K|La8Sr2Ge6O26_675K|Overall
_pd_phase_name
'from C:/RIETVELD/Apatito/SINQ_02/La9.55Si/La955Si6_RT/LA955SI.EXP'
_pd_proc_ls_prof_R_factor        0.0130
_pd_proc_ls_prof_wR_factor       0.0182
_refine_ls_goodness_of_fit_all   1.40
_refine_ls_matrix_type           full
_refine_ls_number_parameters     59
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.09
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            b503374h.txt
_cod_data_source_block           LA8SR2GE6_675K_overall
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (627
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (172 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        627.97675
_cod_database_code               7203770
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.23068(11) -0.01001(14) 0.25 0.8 Uani 0.00825 6
LA La2 0.3333 0.6667 0.00057(19) 0.8 Uani 0.01442 4
GE Ge 0.40013(11) 0.37197(10) 0.25 1.0 Uani 0.00632 6
O O1 0.31505(19) 0.48835(19) 0.25 1.0 Uani 0.01789 6
O O2 0.60172(15) 0.47665(18) 0.25 1.0 Uani 0.01576 6
O O3 0.33934(16) 0.24827(14) 0.06215(12) 1.0 Uani 0.02382 12
O O4 0.0 0.0 0.25 0.969(9) Uani 0.01896 2
SR Sr1 0.23068(11) -0.01001(14) 0.25 0.2 Uani 0.00825 6
SR Sr2 0.33333 0.66667 0.00057(19) 0.2 Uani 0.01443 4
O O5 0.006 0.241 0.613 0.0052(16) Uiso 0.03 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 8.0
GE 6.0
O 26.0
SR 2.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 La1 O3 71.22(5) 3_655 . 1_555 n
O2 La1 O3 85.55(4) 3_655 . 6_555 n
O2 La1 O3 85.55(4) 3_655 . -3_555 n
O2 La1 O3 71.22(5) 3_655 . -4_556 n
O2 La1 O4 150.44(7) 3_655 . 1_555 n
O2 La1 O5 141.63(5) 3_655 . 4_554 n
O2 La1 O5 89.219(21) 3_655 . 5_555 n
O2 La1 O5 90.38(5) 3_655 . 6_554 n
O2 La1 O5 141.63(5) 3_655 . -1_556 n
O2 La1 O5 89.219(21) 3_655 . -2_556 n
O2 La1 O5 90.38(5) 3_655 . -3_556 n
O3 La1 O3 138.30(6) 1_555 . 6_555 n
O3 La1 O3 76.709(23) 1_555 . -3_555 n
O3 La1 O3 63.35(5) 1_555 . -4_556 n
O3 La1 O4 83.76(4) 1_555 . 1_555 n
O3 La1 O5 114.842(29) 1_555 . 4_554 n
O3 La1 O5 120.98(4) 1_555 . 5_555 n
O3 La1 O5 21.918(29) 1_555 . 6_554 n
O3 La1 O5 146.80(5) 1_555 . -1_556 n
O3 La1 O5 57.631(22) 1_555 . -2_556 n
O3 La1 O5 58.663(33) 1_555 . -3_556 n
O3 La1 O3 136.82(8) 6_555 . -3_555 n
O3 La1 O3 76.709(23) 6_555 . -4_556 n
O3 La1 O4 104.18(4) 6_555 . 1_555 n
O3 La1 O5 104.95(5) 6_555 . 4_554 n
O3 La1 O5 21.861(31) 6_555 . 5_555 n
O3 La1 O5 133.86(5) 6_555 . 6_554 n
O3 La1 O5 61.327(33) 6_555 . -1_556 n
O3 La1 O5 158.65(6) 6_555 . -2_556 n
O3 La1 O5 88.342(33) 6_555 . -3_556 n
O3 La1 O3 138.30(6) -3_555 . -4_556 n
O3 La1 O4 104.18(4) -3_555 . 1_555 n
O3 La1 O5 61.327(33) -3_555 . 4_554 n
O3 La1 O5 158.65(6) -3_555 . 5_555 n
O3 La1 O5 88.342(33) -3_555 . 6_554 n
O3 La1 O5 104.95(5) -3_555 . -1_556 n
O3 La1 O5 21.861(31) -3_555 . -2_556 n
O3 La1 O5 133.86(5) -3_555 . -3_556 n
O3 La1 O4 83.76(4) -4_556 . 1_555 n
O3 La1 O5 146.80(5) -4_556 . 4_554 n
O3 La1 O5 57.631(22) -4_556 . 5_555 n
O3 La1 O5 58.663(33) -4_556 . 6_554 n
O3 La1 O5 114.842(29) -4_556 . -1_556 n
O3 La1 O5 120.98(4) -4_556 . -2_556 n
O3 La1 O5 21.918(29) -4_556 . -3_556 n
O4 La1 O5 63.484(24) 1_555 . 4_554 n
O4 La1 O5 90.467(20) 1_555 . 5_555 n
O4 La1 O5 62.586(24) 1_555 . 6_554 n
O4 La1 O5 63.484(24) 1_555 . -1_556 n
O4 La1 O5 90.467(20) 1_555 . -2_556 n
O4 La1 O5 62.586(24) 1_555 . -3_556 n
O5 La1 O5 114.264(35) 4_554 . 5_555 n
O5 La1 O5 106.307(25) 4_554 . 6_554 n
O5 La1 O5 46.746(21) 4_554 . -1_556 n
O5 La1 O5 67.518(14) 4_554 . -2_556 n
O5 La1 O5 126.07(4) 4_554 . -3_556 n
O5 La1 O5 112.41(4) 5_555 . 6_554 n
O5 La1 O5 67.518(14) 5_555 . -1_556 n
O5 La1 O5 178.22(5) 5_555 . -2_556 n
O5 La1 O5 66.739(15) 5_555 . -3_556 n
O5 La1 O5 126.07(4) 6_554 . -1_556 n
O5 La1 O5 66.739(15) 6_554 . -2_556 n
O5 La1 O5 45.678(21) 6_554 . -3_556 n
O5 La1 O5 114.264(35) -1_556 . -2_556 n
O5 La1 O5 106.307(25) -1_556 . -3_556 n
O5 La1 O5 112.41(4) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 137.270(32) -2_565 . 1_555 n
La2 La2 O1 137.274(32) -2_565 . 3_665 n
La2 La2 O1 137.308(32) -2_565 . 5_565 n
La2 La2 O2 44.96(4) -2_565 . 2_554 n
La2 La2 O2 44.95(4) -2_565 . 4_664 n
La2 La2 O2 44.94(4) -2_565 . 6_564 n
La2 La2 Sr2 89.9761 -2_565 . 1_555 n
La2 La2 Sr2 0.0 -2_565 . -2_565 n
La2 La2 Sr2 179.972 -2_565 . -2_566 n
La2 La2 O1 42.717(32) -2_566 . 1_555 n
La2 La2 O1 42.708(32) -2_566 . 3_665 n
La2 La2 O1 42.722(32) -2_566 . 5_565 n
La2 La2 O2 135.07(4) -2_566 . 2_554 n
La2 La2 O2 135.03(4) -2_566 . 4_664 n
La2 La2 O2 135.05(4) -2_566 . 6_564 n
La2 La2 Sr2 89.9761 -2_566 . 1_555 n
La2 La2 Sr2 179.972 -2_566 . -2_565 n
La2 La2 Sr2 0.0 -2_566 . -2_566 n
O1 La2 O1 71.95(5) 1_555 . 3_665 n
O1 La2 O1 71.96(5) 1_555 . 5_565 n
O1 La2 O2 125.28(4) 1_555 . 2_554 n
O1 La2 O2 94.520(33) 1_555 . 4_664 n
O1 La2 O2 154.56(5) 1_555 . 6_564 n
O1 La2 Sr2 56.3864 1_555 . 1_555 n
O1 La2 Sr2 137.269(32) 1_555 . -2_565 n
O1 La2 Sr2 42.716(32) 1_555 . -2_566 n
O1 La2 O1 71.96(5) 3_665 . 5_565 n
O1 La2 O2 154.60(5) 3_665 . 2_554 n
O1 La2 O2 125.27(4) 3_665 . 4_664 n
O1 La2 O2 94.539(33) 3_665 . 6_564 n
O1 La2 Sr2 86.38(4) 3_665 . 1_555 n
O1 La2 Sr2 137.282(32) 3_665 . -2_565 n
O1 La2 Sr2 42.716(32) 3_665 . -2_566 n
O1 La2 O2 94.552(33) 5_565 . 2_554 n
O1 La2 O2 154.58(5) 5_565 . 4_664 n
O1 La2 O2 125.31(4) 5_565 . 6_564 n
O1 La2 Sr2 128.08(4) 5_565 . 1_555 n
O1 La2 Sr2 137.301(32) 5_565 . -2_565 n
O1 La2 Sr2 42.715(32) 5_565 . -2_566 n
O2 La2 O2 75.44(5) 2_554 . 4_664 n
O2 La2 O2 75.45(5) 2_554 . 6_564 n
O2 La2 Sr2 118.340(20) 2_554 . 1_555 n
O2 La2 Sr2 44.95(4) 2_554 . -2_565 n
O2 La2 Sr2 135.06(4) 2_554 . -2_566 n
O2 La2 O2 75.44(5) 4_664 . 6_564 n
O2 La2 Sr2 46.35(4) 4_664 . 1_555 n
O2 La2 Sr2 44.95(4) 4_664 . -2_565 n
O2 La2 Sr2 135.03(4) 4_664 . -2_566 n
O2 La2 Sr2 102.450(24) 6_564 . 1_555 n
O2 La2 Sr2 44.95(4) 6_564 . -2_565 n
O2 La2 Sr2 135.05(4) 6_564 . -2_566 n
Sr2 La2 Sr2 89.9956 1_555 . -2_565 n
Sr2 La2 Sr2 89.9955 1_555 . -2_566 n
Sr2 La2 Sr2 180.0 -2_565 . -2_566 n
O1 Ge O2 113.60(10) 1_555 . 1_555 n
O1 Ge O3 110.90(6) 1_555 . 1_555 n
O1 Ge O3 110.90(6) 1_555 . -4_556 n
O1 Ge Sr1 128.85(7) 1_555 . 1_555 n
O1 Ge Sr1 54.43(6) 1_555 . 3_555 n
O1 Ge Sr2 137.71(4) 1_555 . 2_655 n
O1 Ge Sr2 137.71(4) 1_555 . -1_665 n
O1 Ge O5 88.13(6) 1_555 . 6_554 n
O1 Ge O5 88.13(6) 1_555 . -3_556 n
O2 Ge O3 108.20(7) 1_555 . 1_555 n
O2 Ge O3 108.20(7) 1_555 . -4_556 n
O2 Ge Sr1 117.55(7) 1_555 . 1_555 n
O2 Ge Sr1 168.04(7) 1_555 . 3_555 n
O2 Ge Sr2 48.44(5) 1_555 . 2_655 n
O2 Ge Sr2 48.44(5) 1_555 . -1_665 n
O2 Ge O5 140.47(4) 1_555 . 6_554 n
O2 Ge O5 140.47(4) 1_555 . -3_556 n
O3 Ge O3 104.59(9) 1_555 . -4_556 n
O3 Ge Sr1 52.36(4) 1_555 . 1_555 n
O3 Ge Sr1 78.67(5) 1_555 . 3_555 n
O3 Ge Sr2 111.27(5) 1_555 . 2_655 n
O3 Ge Sr2 60.50(5) 1_555 . -1_665 n
O3 Ge O5 32.55(5) 1_555 . 6_554 n
O3 Ge O5 92.54(6) 1_555 . -3_556 n
O3 Ge Sr1 52.36(4) -4_556 . 1_555 n
O3 Ge Sr1 78.67(5) -4_556 . 3_555 n
O3 Ge Sr2 60.50(5) -4_556 . 2_655 n
O3 Ge Sr2 111.27(5) -4_556 . -1_665 n
O3 Ge O5 92.54(6) -4_556 . 6_554 n
O3 Ge O5 32.55(5) -4_556 . -3_556 n
Sr1 Ge Sr1 74.42(4) 1_555 . 3_555 n
Sr1 Ge Sr2 81.262(19) 1_555 . 2_655 n
Sr1 Ge Sr2 81.262(19) 1_555 . -1_665 n
Sr1 Ge O5 51.400(24) 1_555 . 6_554 n
Sr1 Ge O5 51.400(24) 1_555 . -3_556 n
Sr1 Ge Sr2 139.139(24) 3_555 . 2_655 n
Sr1 Ge Sr2 139.139(24) 3_555 . -1_665 n
Sr1 Ge O5 46.208(23) 3_555 . 6_554 n
Sr1 Ge O5 46.208(23) 3_555 . -3_556 n
Sr2 Ge Sr2 65.43(4) 2_655 . -1_665 n
Sr2 Ge O5 131.208(35) 2_655 . 6_554 n
Sr2 Ge O5 93.024(23) 2_655 . -3_556 n
Sr2 Ge O5 93.024(23) -1_665 . 6_554 n
Sr2 Ge O5 131.208(35) -1_665 . -3_556 n
O5 Ge O5 68.203(34) 6_554 . -3_556 n
La2 O1 La2 94.56(6) 1_555 . -2_566 n
La2 O1 Ge 125.90(4) 1_555 . 1_555 n
La2 O1 Sr1 106.75(4) 1_555 . 3_555 n
La2 O1 Sr2 0.0 1_555 . 1_555 n
La2 O1 Sr2 94.56(6) 1_555 . -2_566 n
La2 O1 Ge 125.88(4) -2_566 . 1_555 n
La2 O1 Sr1 106.77(4) -2_566 . 3_555 n
La2 O1 Sr2 94.57(6) -2_566 . 1_555 n
La2 O1 Sr2 0.0 -2_566 . -2_566 n
Ge O1 Sr1 95.07(7) 1_555 . 3_555 n
Ge O1 Sr2 125.88(4) 1_555 . 1_555 n
Ge O1 Sr2 125.88(4) 1_555 . -2_566 n
Sr1 O1 Sr2 106.76(4) 3_555 . 1_555 n
Sr1 O1 Sr2 106.76(4) 3_555 . -2_566 n
Sr2 O1 Sr2 94.57(6) 1_555 . -2_566 n
La1 O2 La2 116.84(4) 5_665 . 2_655 n
La1 O2 La2 116.84(4) 5_665 . -1_665 n
La1 O2 Ge 123.82(9) 5_665 . 1_555 n
La1 O2 Sr1 0.0 5_665 . 5_665 n
La1 O2 Sr2 116.84(4) 5_665 . 2_655 n
La1 O2 Sr2 116.84(4) 5_665 . -1_665 n
La2 O2 La2 90.09(7) 2_655 . -1_665 n
La2 O2 Ge 101.54(5) 2_655 . 1_555 n
La2 O2 Sr1 116.84(4) 2_655 . 5_665 n
La2 O2 Sr2 0.0 2_655 . 2_655 n
La2 O2 Sr2 90.10(7) 2_655 . -1_665 n
La2 O2 Ge 101.56(5) -1_665 . 1_555 n
La2 O2 Sr1 116.84(4) -1_665 . 5_665 n
La2 O2 Sr2 90.09(7) -1_665 . 2_655 n
La2 O2 Sr2 0.0 -1_665 . -1_665 n
Ge O2 Sr1 123.82(9) 1_555 . 5_665 n
Ge O2 Sr2 101.55(5) 1_555 . 2_655 n
Ge O2 Sr2 101.55(5) 1_555 . -1_665 n
Sr1 O2 Sr2 116.84(4) 5_665 . 2_655 n
Sr1 O2 Sr2 116.84(4) 5_665 . -1_665 n
Sr2 O2 Sr2 90.10(7) 2_655 . -1_665 n
La1 O3 La1 117.67(6) 1_555 . 2_554 n
La1 O3 Ge 95.93(5) 1_555 . 1_555 n
La1 O3 Sr1 0.0 1_555 . 1_555 n
La1 O3 Sr1 117.67(6) 1_555 . 2_554 n
La1 O3 Sr2 102.53(4) 1_555 . -1_665 n
La1 O3 O5 77.07(7) 1_555 . 6_554 n
La1 O3 Ge 140.45(7) 2_554 . 1_555 n
La1 O3 Sr1 117.67(6) 2_554 . 1_555 n
La1 O3 Sr1 0.0 2_554 . 2_554 n
La1 O3 Sr2 102.57(5) 2_554 . -1_665 n
La1 O3 O5 90.52(6) 2_554 . 6_554 n
Ge O3 Sr1 95.93(5) 1_555 . 1_555 n
Ge O3 Sr1 140.45(7) 1_555 . 2_554 n
Ge O3 Sr2 88.71(6) 1_555 . -1_665 n
Ge O3 O5 76.55(6) 1_555 . 6_554 n
Sr1 O3 Sr1 117.67(6) 1_555 . 2_554 n
Sr1 O3 Sr2 102.53(4) 1_555 . -1_665 n
Sr1 O3 O5 77.07(7) 1_555 . 6_554 n
Sr1 O3 Sr2 102.57(5) 2_554 . -1_665 n
Sr1 O3 O5 90.52(6) 2_554 . 6_554 n
Sr2 O3 O5 165.07(7) -1_665 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 Sr1 0.0 1_555 . 1_555 n
La1 O4 Sr1 120.0 1_555 . 3_555 n
La1 O4 Sr1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 3_555 . 1_555 n
La1 O4 Sr1 0.0 3_555 . 3_555 n
La1 O4 Sr1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 5_555 . 1_555 n
La1 O4 Sr1 120.0 5_555 . 3_555 n
La1 O4 Sr1 0.0 5_555 . 5_555 n
Sr1 O4 Sr1 120.0 1_555 . 3_555 n
Sr1 O4 Sr1 120.0 1_555 . 5_555 n
Sr1 O4 Sr1 120.0 3_555 . 5_555 n
Ge Sr1 Ge 165.58(4) 1_555 . 5_555 n
Ge Sr1 O1 163.92(4) 1_555 . 5_555 n
Ge Sr1 O2 66.27(5) 1_555 . 3_655 n
Ge Sr1 O3 31.709(23) 1_555 . 1_555 n
Ge Sr1 O3 107.34(4) 1_555 . 6_555 n
Ge Sr1 O3 107.34(4) 1_555 . -3_555 n
Ge Sr1 O3 31.709(23) 1_555 . -4_556 n
Ge Sr1 O4 84.17(4) 1_555 . 1_555 n
Ge Sr1 Sr1 54.17(4) 1_555 . 3_555 n
Ge Sr1 Sr1 114.17(4) 1_555 . 5_555 n
Ge Sr1 Sr2 134.025(26) 1_555 . 1_545 n
Ge Sr1 Sr2 134.024(26) 1_555 . -2_556 n
Ge Sr1 O5 138.812(32) 1_555 . 4_554 n
Ge Sr1 O5 89.292(26) 1_555 . 5_555 n
Ge Sr1 O5 32.754(19) 1_555 . 6_554 n
Ge Sr1 O5 138.812(32) 1_555 . -1_556 n
Ge Sr1 O5 89.292(26) 1_555 . -2_556 n
Ge Sr1 O5 32.754(19) 1_555 . -3_556 n
Ge Sr1 O1 30.495(27) 5_555 . 5_555 n
Ge Sr1 O2 128.15(5) 5_555 . 3_655 n
Ge Sr1 O3 144.922(29) 5_555 . 1_555 n
Ge Sr1 O3 76.41(4) 5_555 . 6_555 n
Ge Sr1 O3 76.41(4) 5_555 . -3_555 n
Ge Sr1 O3 144.922(29) 5_555 . -4_556 n
Ge Sr1 O4 81.415(34) 5_555 . 1_555 n
Ge Sr1 Sr1 111.415(34) 5_555 . 3_555 n
Ge Sr1 Sr1 51.415(34) 5_555 . 5_555 n
Ge Sr1 Sr2 58.006(21) 5_555 . 1_545 n
Ge Sr1 Sr2 58.006(21) 5_555 . -2_556 n
Ge Sr1 O5 30.715(17) 5_555 . 4_554 n
Ge Sr1 O5 90.821(26) 5_555 . 5_555 n
Ge Sr1 O5 136.111(32) 5_555 . 6_554 n
Ge Sr1 O5 30.715(17) 5_555 . -1_556 n
Ge Sr1 O5 90.821(26) 5_555 . -2_556 n
Ge Sr1 O5 136.111(32) 5_555 . -3_556 n
O1 Sr1 O2 97.65(6) 5_555 . 3_655 n
O1 Sr1 O3 145.451(28) 5_555 . 1_555 n
O1 Sr1 O3 69.75(4) 5_555 . 6_555 n
O1 Sr1 O3 69.75(4) 5_555 . -3_555 n
O1 Sr1 O3 145.451(28) 5_555 . -4_556 n
O1 Sr1 O4 111.91(5) 5_555 . 1_555 n
O1 Sr1 Sr1 141.91(5) 5_555 . 3_555 n
O1 Sr1 Sr1 81.91(5) 5_555 . 5_555 n
O1 Sr1 Sr2 34.194(22) 5_555 . 1_545 n
O1 Sr1 Sr2 34.194(22) 5_555 . -2_556 n
O1 Sr1 O5 54.723(30) 5_555 . 4_554 n
O1 Sr1 O5 90.531(26) 5_555 . 5_555 n
O1 Sr1 O5 155.852(19) 5_555 . 6_554 n
O1 Sr1 O5 54.723(30) 5_555 . -1_556 n
O1 Sr1 O5 90.531(26) 5_555 . -2_556 n
O1 Sr1 O5 155.852(19) 5_555 . -3_556 n
O2 Sr1 O3 71.22(5) 3_655 . 1_555 n
O2 Sr1 O3 85.55(4) 3_655 . 6_555 n
O2 Sr1 O3 85.55(4) 3_655 . -3_555 n
O2 Sr1 O3 71.22(5) 3_655 . -4_556 n
O2 Sr1 O4 150.44(7) 3_655 . 1_555 n
O2 Sr1 Sr1 120.44(7) 3_655 . 3_555 n
O2 Sr1 Sr1 179.5603(5) 3_655 . 5_555 n
O2 Sr1 Sr2 75.70(4) 3_655 . 1_545 n
O2 Sr1 Sr2 75.70(4) 3_655 . -2_556 n
O2 Sr1 O5 141.63(5) 3_655 . 4_554 n
O2 Sr1 O5 89.219(21) 3_655 . 5_555 n
O2 Sr1 O5 90.38(5) 3_655 . 6_554 n
O2 Sr1 O5 141.63(5) 3_655 . -1_556 n
O2 Sr1 O5 89.219(21) 3_655 . -2_556 n
O2 Sr1 O5 90.38(5) 3_655 . -3_556 n
O3 Sr1 O3 138.30(6) 1_555 . 6_555 n
O3 Sr1 O3 76.709(23) 1_555 . -3_555 n
O3 Sr1 O3 63.35(5) 1_555 . -4_556 n
O3 Sr1 O4 83.76(4) 1_555 . 1_555 n
O3 Sr1 Sr1 58.92(4) 1_555 . 3_555 n
O3 Sr1 Sr1 109.14(4) 1_555 . 5_555 n
O3 Sr1 Sr2 112.188(30) 1_555 . 1_545 n
O3 Sr1 Sr2 146.16(4) 1_555 . -2_556 n
O3 Sr1 O5 114.842(29) 1_555 . 4_554 n
O3 Sr1 O5 120.98(4) 1_555 . 5_555 n
O3 Sr1 O5 21.918(29) 1_555 . 6_554 n
O3 Sr1 O5 146.80(5) 1_555 . -1_556 n
O3 Sr1 O5 57.631(22) 1_555 . -2_556 n
O3 Sr1 O5 58.663(33) 1_555 . -3_556 n
O3 Sr1 O3 136.82(8) 6_555 . -3_555 n
O3 Sr1 O3 76.709(23) 6_555 . -4_556 n
O3 Sr1 O4 104.18(4) 6_555 . 1_555 n
O3 Sr1 Sr1 110.45(4) 6_555 . 3_555 n
O3 Sr1 Sr1 94.29(4) 6_555 . 5_555 n
O3 Sr1 Sr2 94.00(5) 6_555 . 1_545 n
O3 Sr1 Sr2 42.93(4) 6_555 . -2_556 n
O3 Sr1 O5 104.95(5) 6_555 . 4_554 n
O3 Sr1 O5 21.861(31) 6_555 . 5_555 n
O3 Sr1 O5 133.86(5) 6_555 . 6_554 n
O3 Sr1 O5 61.327(33) 6_555 . -1_556 n
O3 Sr1 O5 158.65(6) 6_555 . -2_556 n
O3 Sr1 O5 88.342(33) 6_555 . -3_556 n
O3 Sr1 O3 138.30(6) -3_555 . -4_556 n
O3 Sr1 O4 104.18(4) -3_555 . 1_555 n
O3 Sr1 Sr1 110.45(4) -3_555 . 3_555 n
O3 Sr1 Sr1 94.29(4) -3_555 . 5_555 n
O3 Sr1 Sr2 42.93(4) -3_555 . 1_545 n
O3 Sr1 Sr2 94.00(5) -3_555 . -2_556 n
O3 Sr1 O5 61.327(33) -3_555 . 4_554 n
O3 Sr1 O5 158.65(6) -3_555 . 5_555 n
O3 Sr1 O5 88.342(33) -3_555 . 6_554 n
O3 Sr1 O5 104.95(5) -3_555 . -1_556 n
O3 Sr1 O5 21.861(31) -3_555 . -2_556 n
O3 Sr1 O5 133.86(5) -3_555 . -3_556 n
O3 Sr1 O4 83.76(4) -4_556 . 1_555 n
O3 Sr1 Sr1 58.92(4) -4_556 . 3_555 n
O3 Sr1 Sr1 109.14(4) -4_556 . 5_555 n
O3 Sr1 Sr2 146.16(4) -4_556 . 1_545 n
O3 Sr1 Sr2 112.188(30) -4_556 . -2_556 n
O3 Sr1 O5 146.80(5) -4_556 . 4_554 n
O3 Sr1 O5 57.631(22) -4_556 . 5_555 n
O3 Sr1 O5 58.663(33) -4_556 . 6_554 n
O3 Sr1 O5 114.842(29) -4_556 . -1_556 n
O3 Sr1 O5 120.98(4) -4_556 . -2_556 n
O3 Sr1 O5 21.918(29) -4_556 . -3_556 n
O4 Sr1 Sr1 30.0 1_555 . 3_555 n
O4 Sr1 Sr1 30.0 1_555 . 5_555 n
O4 Sr1 Sr2 130.017(35) 1_555 . 1_545 n
O4 Sr1 Sr2 130.017(35) 1_555 . -2_556 n
O4 Sr1 O5 63.484(24) 1_555 . 4_554 n
O4 Sr1 O5 90.467(20) 1_555 . 5_555 n
O4 Sr1 O5 62.586(24) 1_555 . 6_554 n
O4 Sr1 O5 63.484(24) 1_555 . -1_556 n
O4 Sr1 O5 90.467(20) 1_555 . -2_556 n
O4 Sr1 O5 62.586(24) 1_555 . -3_556 n
Sr1 Sr1 Sr1 60.0 3_555 . 5_555 n
Sr1 Sr1 Sr2 150.847(22) 3_555 . 1_545 n
Sr1 Sr1 Sr2 150.847(22) 3_555 . -2_556 n
Sr1 Sr1 O5 90.825(22) 3_555 . 4_554 n
Sr1 Sr1 O5 90.025(22) 3_555 . 5_555 n
Sr1 Sr1 O5 37.069(24) 3_555 . 6_554 n
Sr1 Sr1 O5 90.825(22) 3_555 . -1_556 n
Sr1 Sr1 O5 90.025(22) 3_555 . -2_556 n
Sr1 Sr1 O5 37.069(24) 3_555 . -3_556 n
Sr1 Sr1 Sr2 103.91(4) 5_555 . 1_545 n
Sr1 Sr1 Sr2 103.91(4) 5_555 . -2_556 n
Sr1 Sr1 O5 38.032(24) 5_555 . 4_554 n
Sr1 Sr1 O5 90.785(21) 5_555 . 5_555 n
Sr1 Sr1 O5 90.025(23) 5_555 . 6_554 n
Sr1 Sr1 O5 38.032(24) 5_555 . -1_556 n
Sr1 Sr1 O5 90.784(21) 5_555 . -2_556 n
Sr1 Sr1 O5 90.025(23) 5_555 . -3_556 n
Sr2 Sr1 Sr2 51.09(4) 1_545 . -2_556 n
Sr2 Sr1 O5 66.944(22) 1_545 . 4_554 n
Sr2 Sr1 O5 115.74(4) 1_545 . 5_555 n
Sr2 Sr1 O5 129.343(19) 1_545 . 6_554 n
Sr2 Sr1 O5 87.164(32) 1_545 . -1_556 n
Sr2 Sr1 O5 64.658(23) 1_545 . -2_556 n
Sr2 Sr1 O5 165.63(4) 1_545 . -3_556 n
Sr2 Sr1 O5 87.164(32) -2_556 . 4_554 n
Sr2 Sr1 O5 64.658(23) -2_556 . 5_555 n
Sr2 Sr1 O5 165.63(4) -2_556 . 6_554 n
Sr2 Sr1 O5 66.944(22) -2_556 . -1_556 n
Sr2 Sr1 O5 115.74(4) -2_556 . -2_556 n
Sr2 Sr1 O5 129.343(19) -2_556 . -3_556 n
O5 Sr1 O5 114.264(35) 4_554 . 5_555 n
O5 Sr1 O5 106.307(25) 4_554 . 6_554 n
O5 Sr1 O5 46.746(21) 4_554 . -1_556 n
O5 Sr1 O5 67.518(14) 4_554 . -2_556 n
O5 Sr1 O5 126.07(4) 4_554 . -3_556 n
O5 Sr1 O5 112.41(4) 5_555 . 6_554 n
O5 Sr1 O5 67.518(14) 5_555 . -1_556 n
O5 Sr1 O5 178.22(5) 5_555 . -2_556 n
O5 Sr1 O5 66.739(15) 5_555 . -3_556 n
O5 Sr1 O5 126.07(4) 6_554 . -1_556 n
O5 Sr1 O5 66.739(15) 6_554 . -2_556 n
O5 Sr1 O5 45.678(21) 6_554 . -3_556 n
O5 Sr1 O5 114.264(35) -1_556 . -2_556 n
O5 Sr1 O5 106.307(25) -1_556 . -3_556 n
O5 Sr1 O5 112.41(4) -2_556 . -3_556 n
La2 Sr2 La2 90.0091 1_555 . -2_565 n
La2 Sr2 La2 90.0092 1_555 . -2_566 n
La2 Sr2 Ge 84.4085 1_555 . 2_554 n
La2 Sr2 Ge 140.576(31) 1_555 . 4_664 n
La2 Sr2 Ge 47.521(21) 1_555 . 6_564 n
La2 Sr2 O1 123.615(32) 1_555 . 1_555 n
La2 Sr2 O1 93.63(4) 1_555 . 3_665 n
La2 Sr2 O1 51.95(4) 1_555 . 5_565 n
La2 Sr2 O2 61.655(25) 1_555 . 2_554 n
La2 Sr2 O2 133.685(15) 1_555 . 4_664 n
La2 Sr2 O2 77.585(26) 1_555 . 6_564 n
La2 Sr2 O3 134.745(24) 1_555 . -1_665 n
La2 Sr2 O3 17.807(25) 1_555 . -3_565 n
La2 Sr2 O3 104.345(21) 1_555 . -5_555 n
La2 Sr2 Sr1 30.120(22) 1_555 . 1_565 n
La2 Sr2 Sr1 102.025(6) 1_555 . 3_555 n
La2 Sr2 Sr1 130.978(8) 1_555 . 5_665 n
La2 Sr2 Sr2 90.0001 1_555 . -2_565 n
La2 Sr2 Sr2 90.0001 1_555 . -2_566 n
La2 Sr2 La2 180.0 -2_565 . -2_566 n
La2 Sr2 Ge 57.292(22) -2_565 . 2_554 n
La2 Sr2 Ge 57.277(22) -2_565 . 4_664 n
La2 Sr2 Ge 57.283(22) -2_565 . 6_564 n
La2 Sr2 O1 137.285(32) -2_565 . 1_555 n
La2 Sr2 O1 137.276(32) -2_565 . 3_665 n
La2 Sr2 O1 137.292(32) -2_565 . 5_565 n
La2 Sr2 O2 44.96(4) -2_565 . 2_554 n
La2 Sr2 O2 44.95(4) -2_565 . 4_664 n
La2 Sr2 O2 44.94(4) -2_565 . 6_564 n
La2 Sr2 O3 81.050(31) -2_565 . -1_665 n
La2 Sr2 O3 81.061(31) -2_565 . -3_565 n
La2 Sr2 O3 81.065(31) -2_565 . -5_555 n
La2 Sr2 Sr1 115.548(19) -2_565 . 1_565 n
La2 Sr2 Sr1 115.552(19) -2_565 . 3_555 n
La2 Sr2 Sr1 115.537(19) -2_565 . 5_665 n
La2 Sr2 Sr2 0.0 -2_565 . -2_565 n
La2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La2 Sr2 Ge 122.724(22) -2_566 . 2_554 n
La2 Sr2 Ge 122.709(22) -2_566 . 4_664 n
La2 Sr2 Ge 122.715(22) -2_566 . 6_564 n
La2 Sr2 O1 42.717(32) -2_566 . 1_555 n
La2 Sr2 O1 42.708(32) -2_566 . 3_665 n
La2 Sr2 O1 42.723(32) -2_566 . 5_565 n
La2 Sr2 O2 135.06(4) -2_566 . 2_554 n
La2 Sr2 O2 135.05(4) -2_566 . 4_664 n
La2 Sr2 O2 135.04(4) -2_566 . 6_564 n
La2 Sr2 O3 98.933(31) -2_566 . -1_665 n
La2 Sr2 O3 98.944(31) -2_566 . -3_565 n
La2 Sr2 O3 98.948(31) -2_566 . -5_555 n
La2 Sr2 Sr1 64.457(19) -2_566 . 1_565 n
La2 Sr2 Sr1 64.461(19) -2_566 . 3_555 n
La2 Sr2 Sr1 64.446(19) -2_566 . 5_665 n
La2 Sr2 Sr2 180.0 -2_566 . -2_565 n
La2 Sr2 Sr2 0.0 -2_566 . -2_566 n
Ge Sr2 Ge 93.545(30) 2_554 . 4_664 n
Ge Sr2 Ge 93.545(30) 2_554 . 6_564 n
Ge Sr2 O1 97.08(4) 2_554 . 1_555 n
Ge Sr2 O1 165.40(5) 2_554 . 3_665 n
Ge Sr2 O1 95.759(25) 2_554 . 5_565 n
Ge Sr2 O2 30.009(31) 2_554 . 2_554 n
Ge Sr2 O2 63.88(4) 2_554 . 4_664 n
Ge Sr2 O2 99.13(5) 2_554 . 6_564 n
Ge Sr2 O3 124.30(4) 2_554 . -1_665 n
Ge Sr2 O3 92.491(32) 2_554 . -3_565 n
Ge Sr2 O3 30.795(22) 2_554 . -5_555 n
Ge Sr2 Sr1 111.381(19) 2_554 . 1_565 n
Ge Sr2 Sr1 61.305(14) 2_554 . 3_555 n
Ge Sr2 Sr1 144.567(22) 2_554 . 5_665 n
Ge Sr2 Sr2 57.284(22) 2_554 . -2_565 n
Ge Sr2 Sr2 122.716(22) 2_554 . -2_566 n
Ge Sr2 Ge 93.545(30) 4_664 . 6_564 n
Ge Sr2 O1 95.759(25) 4_664 . 1_555 n
Ge Sr2 O1 97.08(4) 4_664 . 3_665 n
Ge Sr2 O1 165.40(5) 4_664 . 5_565 n
Ge Sr2 O2 99.13(5) 4_664 . 2_554 n
Ge Sr2 O2 30.009(31) 4_664 . 4_664 n
Ge Sr2 O2 63.88(4) 4_664 . 6_564 n
Ge Sr2 O3 30.795(22) 4_664 . -1_665 n
Ge Sr2 O3 124.30(4) 4_664 . -3_565 n
Ge Sr2 O3 92.490(32) 4_664 . -5_555 n
Ge Sr2 Sr1 144.567(22) 4_664 . 1_565 n
Ge Sr2 Sr1 111.380(19) 4_664 . 3_555 n
Ge Sr2 Sr1 61.305(14) 4_664 . 5_665 n
Ge Sr2 Sr2 57.284(22) 4_664 . -2_565 n
Ge Sr2 Sr2 122.716(22) 4_664 . -2_566 n
Ge Sr2 O1 165.40(5) 6_564 . 1_555 n
Ge Sr2 O1 95.759(25) 6_564 . 3_665 n
Ge Sr2 O1 97.08(4) 6_564 . 5_565 n
Ge Sr2 O2 63.88(4) 6_564 . 2_554 n
Ge Sr2 O2 99.13(5) 6_564 . 4_664 n
Ge Sr2 O2 30.009(31) 6_564 . 6_564 n
Ge Sr2 O3 92.490(32) 6_564 . -1_665 n
Ge Sr2 O3 30.796(22) 6_564 . -3_565 n
Ge Sr2 O3 124.30(4) 6_564 . -5_555 n
Ge Sr2 Sr1 61.305(14) 6_564 . 1_565 n
Ge Sr2 Sr1 144.567(22) 6_564 . 3_555 n
Ge Sr2 Sr1 111.380(19) 6_564 . 5_665 n
Ge Sr2 Sr2 57.284(22) 6_564 . -2_565 n
Ge Sr2 Sr2 122.716(22) 6_564 . -2_566 n
O1 Sr2 O1 71.96(5) 1_555 . 3_665 n
O1 Sr2 O1 71.96(5) 1_555 . 5_565 n
O1 Sr2 O2 125.28(4) 1_555 . 2_554 n
O1 Sr2 O2 94.537(33) 1_555 . 4_664 n
O1 Sr2 O2 154.58(5) 1_555 . 6_564 n
O1 Sr2 O3 89.78(4) 1_555 . -1_665 n
O1 Sr2 O3 138.12(5) 1_555 . -3_565 n
O1 Sr2 O3 66.55(4) 1_555 . -5_555 n
O1 Sr2 Sr1 105.24(4) 1_555 . 1_565 n
O1 Sr2 Sr1 39.05(4) 1_555 . 3_555 n
O1 Sr2 Sr1 64.10(4) 1_555 . 5_665 n
O1 Sr2 Sr2 137.284(32) 1_555 . -2_565 n
O1 Sr2 Sr2 42.716(32) 1_555 . -2_566 n
O1 Sr2 O1 71.96(5) 3_665 . 5_565 n
O1 Sr2 O2 154.58(5) 3_665 . 2_554 n
O1 Sr2 O2 125.28(4) 3_665 . 4_664 n
O1 Sr2 O2 94.537(33) 3_665 . 6_564 n
O1 Sr2 O3 66.55(4) 3_665 . -1_665 n
O1 Sr2 O3 89.78(4) 3_665 . -3_565 n
O1 Sr2 O3 138.12(5) 3_665 . -5_555 n
O1 Sr2 Sr1 64.10(4) 3_665 . 1_565 n
O1 Sr2 Sr1 105.24(4) 3_665 . 3_555 n
O1 Sr2 Sr1 39.05(4) 3_665 . 5_665 n
O1 Sr2 Sr2 137.284(32) 3_665 . -2_565 n
O1 Sr2 Sr2 42.716(32) 3_665 . -2_566 n
O1 Sr2 O2 94.537(33) 5_565 . 2_554 n
O1 Sr2 O2 154.58(5) 5_565 . 4_664 n
O1 Sr2 O2 125.28(4) 5_565 . 6_564 n
O1 Sr2 O3 138.12(5) 5_565 . -1_665 n
O1 Sr2 O3 66.55(4) 5_565 . -3_565 n
O1 Sr2 O3 89.78(4) 5_565 . -5_555 n
O1 Sr2 Sr1 39.05(4) 5_565 . 1_565 n
O1 Sr2 Sr1 64.10(4) 5_565 . 3_555 n
O1 Sr2 Sr1 105.24(4) 5_565 . 5_665 n
O1 Sr2 Sr2 137.284(32) 5_565 . -2_565 n
O1 Sr2 Sr2 42.716(32) 5_565 . -2_566 n
O2 Sr2 O2 75.45(5) 2_554 . 4_664 n
O2 Sr2 O2 75.45(5) 2_554 . 6_564 n
O2 Sr2 O3 125.93(6) 2_554 . -1_665 n
O2 Sr2 O3 64.90(4) 2_554 . -3_565 n
O2 Sr2 O3 60.491(32) 2_554 . -5_555 n
O2 Sr2 Sr1 91.702(32) 2_554 . 1_565 n
O2 Sr2 Sr1 86.853(30) 2_554 . 3_555 n
O2 Sr2 Sr1 160.18(5) 2_554 . 5_665 n
O2 Sr2 Sr2 44.95(4) 2_554 . -2_565 n
O2 Sr2 Sr2 135.05(4) 2_554 . -2_566 n
O2 Sr2 O2 75.45(5) 4_664 . 6_564 n
O2 Sr2 O3 60.491(32) 4_664 . -1_665 n
O2 Sr2 O3 125.93(6) 4_664 . -3_565 n
O2 Sr2 O3 64.90(4) 4_664 . -5_555 n
O2 Sr2 Sr1 160.18(5) 4_664 . 1_565 n
O2 Sr2 Sr1 91.702(32) 4_664 . 3_555 n
O2 Sr2 Sr1 86.853(30) 4_664 . 5_665 n
O2 Sr2 Sr2 44.95(4) 4_664 . -2_565 n
O2 Sr2 Sr2 135.05(4) 4_664 . -2_566 n
O2 Sr2 O3 64.90(4) 6_564 . -1_665 n
O2 Sr2 O3 60.491(32) 6_564 . -3_565 n
O2 Sr2 O3 125.93(6) 6_564 . -5_555 n
O2 Sr2 Sr1 86.853(30) 6_564 . 1_565 n
O2 Sr2 Sr1 160.18(5) 6_564 . 3_555 n
O2 Sr2 Sr1 91.702(32) 6_564 . 5_665 n
O2 Sr2 Sr2 44.95(4) 6_564 . -2_565 n
O2 Sr2 Sr2 135.05(4) 6_564 . -2_566 n
O3 Sr2 O3 117.630(16) -1_665 . -3_565 n
O3 Sr2 O3 117.630(16) -1_665 . -5_555 n
O3 Sr2 Sr1 119.804(27) -1_665 . 1_565 n
O3 Sr2 Sr1 121.878(31) -1_665 . 3_555 n
O3 Sr2 Sr1 34.505(19) -1_665 . 5_665 n
O3 Sr2 Sr2 81.059(31) -1_665 . -2_565 n
O3 Sr2 Sr2 98.941(31) -1_665 . -2_566 n
O3 Sr2 O3 117.631(16) -3_565 . -5_555 n
O3 Sr2 Sr1 34.505(19) -3_565 . 1_565 n
O3 Sr2 Sr1 119.804(27) -3_565 . 3_555 n
O3 Sr2 Sr1 121.878(31) -3_565 . 5_665 n
O3 Sr2 Sr2 81.059(31) -3_565 . -2_565 n
O3 Sr2 Sr2 98.941(31) -3_565 . -2_566 n
O3 Sr2 Sr1 121.878(31) -5_555 . 1_565 n
O3 Sr2 Sr1 34.505(19) -5_555 . 3_555 n
O3 Sr2 Sr1 119.803(27) -5_555 . 5_665 n
O3 Sr2 Sr2 81.059(31) -5_555 . -2_565 n
O3 Sr2 Sr2 98.941(31) -5_555 . -2_566 n
Sr1 Sr2 Sr1 102.772(23) 1_565 . 3_555 n
Sr1 Sr2 Sr1 102.772(23) 1_565 . 5_665 n
Sr1 Sr2 Sr2 115.546(19) 1_565 . -2_565 n
Sr1 Sr2 Sr2 64.455(19) 1_565 . -2_566 n
Sr1 Sr2 Sr1 102.772(23) 3_555 . 5_665 n
Sr1 Sr2 Sr2 115.545(19) 3_555 . -2_565 n
Sr1 Sr2 Sr2 64.455(19) 3_555 . -2_566 n
Sr1 Sr2 Sr2 115.545(19) 5_665 . -2_565 n
Sr1 Sr2 Sr2 64.454(19) 5_665 . -2_566 n
Sr2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La1 O5 La1 111.947(32) 2_555 . 3_555 n
La1 O5 La1 104.899(34) 2_555 . 4_555 n
La1 O5 Ge 95.846(31) 2_555 . 2_555 n
La1 O5 O3 81.02(7) 2_555 . 2_555 n
La1 O5 Sr1 0.0 2_555 . 2_555 n
La1 O5 Sr1 111.947(32) 2_555 . 3_555 n
La1 O5 Sr1 104.899(34) 2_555 . 4_555 n
La1 O5 La1 113.783(34) 3_555 . 4_555 n
La1 O5 Ge 124.493(26) 3_555 . 2_555 n
La1 O5 O3 67.62(5) 3_555 . 2_555 n
La1 O5 Sr1 111.947(32) 3_555 . 2_555 n
La1 O5 Sr1 0.0 3_555 . 3_555 n
La1 O5 Sr1 113.783(34) 3_555 . 4_555 n
La1 O5 Ge 103.077(30) 4_555 . 2_555 n
La1 O5 O3 172.19(7) 4_555 . 2_555 n
La1 O5 Sr1 104.899(34) 4_555 . 2_555 n
La1 O5 Sr1 113.783(34) 4_555 . 3_555 n
La1 O5 Sr1 0.0 4_555 . 4_555 n
Ge O5 O3 70.90(6) 2_555 . 2_555 n
Ge O5 Sr1 95.846(31) 2_555 . 2_555 n
Ge O5 Sr1 124.493(26) 2_555 . 3_555 n
Ge O5 Sr1 103.077(30) 2_555 . 4_555 n
O3 O5 Sr1 81.02(7) 2_555 . 2_555 n
O3 O5 Sr1 67.62(5) 2_555 . 3_555 n
O3 O5 Sr1 172.19(7) 2_555 . 4_555 n
Sr1 O5 Sr1 111.947(32) 2_555 . 3_555 n
Sr1 O5 Sr1 104.899(34) 2_555 . 4_555 n
Sr1 O5 Sr1 113.783(34) 3_555 . 4_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.0614(16) . 3_555 n
La1 La1 4.0614(16) . 5_555 n
La1 Ge 3.2959(15) . 1_555 n
La1 Ge 3.4184(16) . 5_555 n
La1 O1 2.7916(21) . 5_555 n
La1 O2 2.5224(17) . 3_655 n
La1 O3 2.6241(17) . 1_555 n
La1 O3 2.4626(9) . 6_555 n
La1 O3 2.4626(9) . -3_555 n
La1 O3 2.6241(17) . -4_556 n
La1 O4 2.3448(9) . 1_555 n
La1 Sr1 4.3533(5) . 2_554 n
La1 Sr1 4.3533(5) . 2_555 n
La1 Sr1 4.0614(16) . 3_555 n
La1 Sr1 4.0614(16) . 5_555 n
La1 Sr1 4.3533(5) . 6_554 n
La1 Sr1 4.3533(5) . 6_555 n
La1 Sr2 4.2431(12) . 1_545 n
La1 Sr2 4.3616(12) . 2_655 n
La1 Sr2 4.3616(12) . -1_665 n
La1 Sr2 4.2431(12) . -2_556 n
La1 O5 2.5333(11) . 4_554 n
La1 O5 2.66320(16) . 5_555 n
La1 O5 2.5893(11) . 6_554 n
La1 O5 2.5333(11) . -1_556 n
La1 O5 2.66320(16) . -2_556 n
La1 O5 2.5893(11) . -3_556 n
La2 La2 3.6763(28) . -2_565 n
La2 La2 3.6595(28) . -2_566 n
La2 Ge 3.4009(11) . 2_554 n
La2 Ge 3.4014(11) . 4_664 n
La2 Ge 3.4006(11) . 6_564 n
La2 O1 2.4907(14) . 1_555 n
La2 O1 2.4904(14) . 3_665 n
La2 O1 2.4900(14) . 5_565 n
La2 O2 2.5970(15) . 2_554 n
La2 O2 2.5977(15) . 4_664 n
La2 O2 2.5972(15) . 6_564 n
La2 O3 2.9611(14) . -1_665 n
La2 O3 2.9601(14) . -3_565 n
La2 O3 2.9608(14) . -5_555 n
La2 Sr1 4.2426(12) . 1_565 n
La2 Sr1 4.3620(12) . 2_554 n
La2 Sr1 4.2432(12) . 3_555 n
La2 Sr1 4.3617(12) . 4_664 n
La2 Sr1 4.2435(12) . 5_665 n
La2 Sr1 4.3611(12) . 6_564 n
La2 Sr2 0.00057 . 1_555 n
La2 Sr2 3.6763(28) . -2_565 n
La2 Sr2 3.6595(28) . -2_566 n
Ge La1 3.2959(15) . 1_555 n
Ge La1 3.4184(16) . 3_555 n
Ge La2 3.4006(11) . 2_655 n
Ge La2 3.4014(11) . -1_665 n
Ge O1 1.7415(13) . 1_555 n
Ge O2 1.7362(16) . 1_555 n
Ge O3 1.7417(10) . 1_555 n
Ge O3 1.7417(10) . -4_556 n
Ge Sr1 3.2959(15) . 1_555 n
Ge Sr1 3.4184(16) . 3_555 n
Ge Sr1 3.7751(13) . 5_665 n
Ge Sr2 3.7841(9) . 1_555 n
Ge Sr2 3.4010(11) . 2_655 n
Ge Sr2 3.4010(11) . -1_665 n
Ge Sr2 3.7841(9) . -2_566 n
Ge O5 1.7925(8) . 6_554 n
Ge O5 1.7925(8) . -3_556 n
O1 La1 2.7916(21) . 3_555 n
O1 La2 2.4907(14) . 1_555 n
O1 La2 2.4904(14) . -2_566 n
O1 Ge 1.7415(13) . 1_555 n
O1 Sr1 2.7916(21) . 3_555 n
O1 Sr2 2.4904(14) . 1_555 n
O1 Sr2 2.4904(14) . -2_566 n
O2 La1 2.5224(17) . 5_665 n
O2 La2 2.5972(15) . 2_655 n
O2 La2 2.5977(15) . -1_665 n
O2 Ge 1.7362(16) . 1_555 n
O2 Sr1 2.5224(17) . 5_665 n
O2 Sr2 2.5973(15) . 2_655 n
O2 Sr2 2.5973(15) . -1_665 n
O3 La1 2.6241(17) . 1_555 n
O3 La1 2.4626(9) . 2_554 n
O3 La2 2.9611(14) . -1_665 n
O3 Ge 1.7417(10) . 1_555 n
O3 Sr1 2.6241(17) . 1_555 n
O3 Sr1 2.4626(9) . 2_554 n
O3 Sr2 2.9607(14) . -1_665 n
O3 O5 0.9917(13) . 6_554 n
O4 La1 2.3448(9) . 1_555 n
O4 La1 2.3448(9) . 3_555 n
O4 La1 2.3448(9) . 5_555 n
O4 Sr1 2.3448(9) . 1_555 n
O4 Sr1 2.3448(9) . 3_555 n
O4 Sr1 2.3448(9) . 5_555 n
Sr1 La1 4.3533(5) . 2_554 n
Sr1 La1 4.3533(5) . 2_555 n
Sr1 La1 4.0614(16) . 3_555 n
Sr1 La1 4.0614(16) . 5_555 n
Sr1 La1 4.3533(5) . 6_554 n
Sr1 La1 4.3533(5) . 6_555 n
Sr1 La2 4.2426(12) . 1_545 n
Sr1 La2 4.3611(12) . 2_655 n
Sr1 La2 4.3617(12) . -1_665 n
Sr1 La2 4.2432(12) . -2_556 n
Sr1 Ge 3.2959(15) . 1_555 n
Sr1 Ge 3.7751(13) . 3_655 n
Sr1 Ge 3.4184(16) . 5_555 n
Sr1 O1 2.7916(21) . 5_555 n
Sr1 O2 2.5224(17) . 3_655 n
Sr1 O3 2.6241(17) . 1_555 n
Sr1 O3 2.4626(9) . 6_555 n
Sr1 O3 2.4626(9) . -3_555 n
Sr1 O3 2.6241(17) . -4_556 n
Sr1 O4 2.3448(9) . 1_555 n
Sr1 Sr1 4.3533(5) . 2_554 n
Sr1 Sr1 4.3533(5) . 2_555 n
Sr1 Sr1 4.0614(16) . 3_555 n
Sr1 Sr1 4.0614(16) . 5_555 n
Sr1 Sr1 4.3533(5) . 6_554 n
Sr1 Sr1 4.3533(5) . 6_555 n
Sr1 Sr2 4.2431(12) . 1_545 n
Sr1 Sr2 4.3616(12) . 2_655 n
Sr1 Sr2 4.3616(12) . -1_665 n
Sr1 Sr2 4.2431(12) . -2_556 n
Sr1 O5 2.5333(11) . 4_554 n
Sr1 O5 2.66320(16) . 5_555 n
Sr1 O5 2.5893(11) . 6_554 n
Sr1 O5 2.5333(11) . -1_556 n
Sr1 O5 2.66320(16) . -2_556 n
Sr1 O5 2.5893(11) . -3_556 n
Sr2 La1 4.2431(12) . 1_565 n
Sr2 La1 4.3616(12) . 2_554 n
Sr2 La1 4.2431(12) . 3_555 n
Sr2 La1 4.3616(12) . 4_664 n
Sr2 La1 4.2431(12) . 5_665 n
Sr2 La1 4.3616(12) . 6_564 n
Sr2 La2 0.00057 . 1_555 n
Sr2 La2 3.6763(28) . -2_565 n
Sr2 La2 3.6595(28) . -2_566 n
Sr2 Ge 3.7841(9) . 1_555 n
Sr2 Ge 3.4010(11) . 2_554 n
Sr2 Ge 3.7841(9) . 3_665 n
Sr2 Ge 3.4010(11) . 4_664 n
Sr2 Ge 3.7841(9) . 5_565 n
Sr2 Ge 3.4010(11) . 6_564 n
Sr2 O1 2.4904(14) . 1_555 n
Sr2 O1 2.4904(14) . 3_665 n
Sr2 O1 2.4904(14) . 5_565 n
Sr2 O2 2.5973(15) . 2_554 n
Sr2 O2 2.5973(15) . 4_664 n
Sr2 O2 2.5973(15) . 6_564 n
Sr2 O3 2.9607(14) . -1_665 n
Sr2 O3 2.9607(14) . -3_565 n
Sr2 O3 2.9607(14) . -5_555 n
Sr2 Sr1 4.2431(12) . 1_565 n
Sr2 Sr1 4.3616(12) . 2_554 n
Sr2 Sr1 4.2431(12) . 3_555 n
Sr2 Sr1 4.3616(12) . 4_664 n
Sr2 Sr1 4.2431(12) . 5_665 n
Sr2 Sr1 4.3616(12) . 6_564 n
Sr2 Sr2 3.6763(28) . -2_565 n
Sr2 Sr2 3.6595(28) . -2_566 n
O5 La1 2.5893(11) . 2_555 n
O5 La1 2.66320(16) . 3_555 n
O5 La1 2.5333(11) . 4_555 n
O5 Ge 1.7925(8) . 2_555 n
O5 O3 0.9917(13) . 2_555 n
O5 Sr1 2.5893(11) . 2_555 n
O5 Sr1 2.66320(16) . 3_555 n
O5 Sr1 2.5333(11) . 4_555 n
O5 O5 2.01000(12) . -4_557 n
loop_
_pd_block_diffractogram_id
;
2004-06-11T10:29|LA8SR2GE6_675K_H_01|La8Sr2Ge6O26_675K|TOF_675k
2004-06-11T10:29|LA8SR2GE6_675K_H_02|La8Sr2Ge6O26_675K|TOF_675K
;
loop_
_pd_phase_block_id
2004-06-11T10:29|LA8SR2GE6_675K_phase1|La8Sr2Ge6O26_675K||
